Materials and Design 32 (2011) 2644–2649
Contents lists available at ScienceDirect
Materials and Design journal homepage: www.elsevier.com/locate/matdes
Role of zirconia ﬁller on friction and dry sliding wear behaviour of bismaleimide nanocomposites R.V. Kurahatti a, A.O. Surendranathan b, S. Srivastava c, N. Singh c, A.V. Ramesh Kumar c, B. Suresha d,⇑ a
Department of Mechanical Engineering, Basaveshwar Engineering College, Bagalkot 587 102, India National Institute of Technology Karnataka, Surathkal-575 025, India c Defence Materials and Stores Research & Development Establishment, Kanpur 280 013, India d Department of Mechanical Engineering, The National Institute of Engineering, Mysore 570 008, India b
a r t i c l e
i n f o
Article history: Received 23 August 2010 Accepted 15 January 2011 Available online 22 January 2011 Keywords: A. Nanomaterials E. Wear G. Scanning electron microscopy
a b s t r a c t This paper discusses the friction and dry sliding wear behaviour of nano-zirconia (nano-ZrO2) ﬁlled bismleimide (BMI) composites. Nano-ZrO2 ﬁlled BMI composites, containing 0.5, 1, 5 and 10 wt.% were prepared using high shear mixer. The inﬂuence of these particles on the microhardness, friction and dry sliding wear behaviour were measured with microhardness tester and pin-on-disc wear apparatus. The experimental results indicated that the frictional coefﬁcient and speciﬁc wear rate of BMI can be reduced at rather low concentration of nano-ZrO2. The lowest speciﬁc wear rate of 4 106 mm3/Nm was observed for 5 wt.% nano-ZrO2 ﬁlled composite which is decreased by 78% as compared to the neat BMI. The incorporation of nano-ZrO2 particles leads to an increased hardness of BMI and wear performance of the composites shows good correlation with the hardness up to 5 wt.% of ﬁller loading. The results have been supplemented with scanning electron micrographs to help understand the possible wear mechanisms. Ó 2011 Elsevier Ltd All rights reserved.
1. Introduction In recent years, nanoparticles have been used as ﬁllers in polymeric composites for improving the tribological performance of the materials (nano-Al2O3/polyphenylene sulﬁde (PPS), nanoZnO/polytetraﬂuroethylene (PTFE), nano-TiO2/epoxy, nano-SiO2/ polyarylate, nano-ZrO2/polyetheretherketone (PEEK), nano-Si3N4/ bismaleimide). Besides, ﬁber reinforcement is a traditional way to produce high performance composites materials. When nanoparticles are incorporated, both microstructure and properties of the composites can be optimized. Zhang et al. [1,2] systematically studied the wear resistance of epoxy ﬁlled with short carbon ﬁber, graphite, PTFE and nano-TiO2 under different sliding conditions. The spherical nano-TiO2 was able to apparently reduce the friction coefﬁcient during sliding and consequently to reduce the shear stress, contact temperature and wear rate of ﬁber reinforced epoxy composites. Based on microscopic observations of the worn surfaces, a positive rolling effect of the nanoparticles between the materials pair was proposed, which led to remarkable reduction of friction coefﬁcient. In order to improve the friction and wear behaviour of polymeric materials, one typical concept is to reduce their adhesion to the counterpart material and to enhance their
⇑ Corresponding author. Tel.: +91 821 2480475; fax: +91 821 2485802. E-mail addresses: [email protected]
, [email protected]
(B. Suresha). 0261-3069/$ - see front matter Ó 2011 Elsevier Ltd All rights reserved. doi:10.1016/j.matdes.2011.01.030
mechanical properties. This can be achieved quite successfully by using inorganic ﬁllers. Ng et al.  veriﬁed that nanoparticles can remarkably reduce the wear rate, while micron sized particles cannot. Rong et al.  conformed that the dispersion state of the nanoparticles and micro-structural homogeneity of the ﬁllers improved the wear resistance signiﬁcantly. The way of nanoparticle incorporation must be considered as a very important key point to receive the desired material properties. The composites containing nanoparticles exhibit the best antiwear property by forming a uniform and tenacious transfer ﬁlm on the ring surface. Especially, for PEEK/ZrO2 nanocomposites. Zhang et al. [5,6] concluded that the addition of the grafted nanosilica into epoxy signiﬁcantly reduced wear rate and frictional coefﬁcient of the matrix at low ﬁller loading. Compared with the cases of microsized silica and untreated nanosilica, the employment of grafted nanosilica provided the composites with much higher tribological performance. Wang et al.  presented experimental results which indicate that the ability of nano-ZrO2 to improve the tribological behaviour is increased with decreasing particle size of the ﬁller. The wear rate of larger particle size was high because the composite transfer ﬁlm had poor adhesion to the counterface. On the other hand, the wear-resistant PEEK composite which was ﬁlled with small size ZrO2 particles transferred well to the counterface and its transfer ﬁlm was thin, uniform and adhered strongly to the counterface [1,2,7]. In the same way, the bismaleimide nanocomposites with surface-modiﬁed SiO2 nanoparticles showed
R.V. Kurahatti et al. / Materials and Design 32 (2011) 2644–2649
better wear resistance and lower frictional coefﬁcient than composites with the unmodiﬁed nanoparticles SiO2 . The chemical treatment of the particle surface may further enhance the composite properties by improving the ﬁller-matrix coupling quality . For purposes of maximizing the use of nanoparticles, hybrid particulate ﬁllers were employed in epoxy nanocomposites. In the work by Wetzel et al. , various amounts of micro- and nanoscale particles (calcium silicate CaSiO3, 4–15 lm; alumina Al2O3, 13 nm) were introduced into epoxy. Choosing the nanocomposite with the highest performance as a matrix, conventional CaSiO3 microparticles were further added in order to achieve additional enhancements in the properties. As a result, synergistic effects were found in the form of a further increase in wear resistance and stiffness. One of the distinct advantages of nanocomposites over microcomposites lies in that the performance improvement is often acquired at relatively low concentration of the nano-ﬁllers. Polymer composites must withstand high mechanical loads; it is usually reinforced with ﬁllers. The addition of different ﬁllers favorably stiffens the material and may also increase the strength under certain load conditions. However, some micro-ﬁllers have a detrimental effect on the abrasion resistance [11,12]. In fact, it was veriﬁed experimentally by several research groups all over the world [9–13] that nanoparticles of metallic or inorganic type prove the ability to reinforce effectively thermoplastic and also thermosetting polymer matrices. Speciﬁcally, the reinforcement covers improvements of the ﬂexural modulus without loosing ﬂexural strength. This effect is at the same time accompanied by improvements in fracture toughness and impact energy which, however, depend strongly on the ﬁller volume content . Only the nanoﬁller induced micromechanical deformation processes can be responsible for this behaviour . However, the nanocomposite can only be effective, if the nanoparticles are well dispersed in the surrounding polymer matrix. It has been shown, that a considerable improvement in the mechanical and tribological properties can be achieved at very low ﬁller volume content (<10%). The method of addition of nanoparticles must be considered as an important key point to get the desired material properties. Bismaleimide (BMI) resin systems are derived from a variety of different starting chemical compounds, with some commonality in the ﬁnal resin (Fig. 1). In the formulas, 4 and 40 denote the position of substituted maleimide group in the ﬁrst and second benzene rings respectively. o and o0 denote the position of allyl group, ortho (o) with respect to the –OH group in the ﬁrst and second benzene
rings respectively. This BMI is synthesized from 4,40 bismaleimidodiphenylmethane and maleic acid anhydride, with the synthesis being followed by cyclodehydration. It is the main building block of almost all commercially available BMI resins. BMI was synthesized according to the method for synthesis of allyl ether novlak described in . These resin systems exhibit a high glass transition temperature (Tg) relative to post cure temperature, dimensionally stable at elevated temperatures (>260 °C) and have low ﬂammability characteristics. In addition, they handle well in processing as a hot melt, exhibit good humidity resistance, good toughness and excellent mechanical properties at both ambient and elevated temperatures. Many modiﬁed BMI resin systems have been developed. Among them a two-component high performance resin system based on BDM and o,o0 -diallyl bisphenol A (DBA), coded as BDM/DBA has been proved to have outstanding toughness, good humidity resistance, excellent thermal and mechanical properties . Hence, the BDM/DBA resin was chosen as the base resin in the present work. Nanocomposites using thermoplastic polymers are well known for improving the mechanical, electrical, thermal and insulating properties. However, nanocomposites using thermosetting polymers have not been studied extensively. Lin et al.  investigated the effect of interfacial adhesion between Kevlar-ﬁber and BMI matrix. Liu et al.  studied the micro-tribological behaviour of BMI/ carbon nanotubes (CNTs) nanocomposite. Although, a good amount of work has been reported on the sliding wear behaviour of particulate ﬁlled polymer matrix composites as discussed earlier in this section, no literature could be cited on the sliding wear aspect of ZrO2 ﬁlled BMI nanocomposites. In this study, we have developed a new type of ZrO2 nanoparticles ﬁlled BMI composites. A high shear mixing procedure was used to uniformly disperse the ZrO2 nanoparticles into the BMI resin system. Effect of incorporation of ZrO2 nanoparticles on microstructure, hardness, friction and dry sliding wear has been determined and analyzed. 2. Experimental procedure 2.1. Materials 4,40 -Bismaleimidodiphenylmethane (BDM) and o,o0 -diallylbisphenol A (BA) were supplied by ABR Organics Limited, Hyderabad (India), Zirconia (ZrO2) nanoparticles were purchased from Sigma Aldrich, Bangalore (India).
Fig. 1. Structural formulas. Top: 4,40 -bismaleimidodiphenylmethane (BDM); Bottom: o,o0 -diallyl-bisphenol A (BA).
R.V. Kurahatti et al. / Materials and Design 32 (2011) 2644–2649
stirring for another 2 h to obtain a homogeneous suspension. Then the suspension was added into BDM at 130 °C with thorough stirring, and kept at that temperature for 15 min. After that the resultant mixture was poured into a preheated mold and degassed in a vacuum oven at 130 °C for 1 h. The mixture was cured in the oven as per the oven temperature proﬁle in Fig. 3a. After curing, the panels were removed from the molds. Then the panels were again put in between the glass plates and clamped together. No rubber o-ring was used this time to eliminate the possibility of warp of the panel during post curing. The panels were again put back into the oven for post curing. The post cure cycle is shown in Fig. 3b. After post curing, the glass plates were removed and the panels were put in the desiccator for storage before use. 2.3. Characterization
Fig. 2. Microstructure of zirconia nanoparticles.
Fig. 3a. Curing cycle.
The microhardness of samples was determined by conducting ﬁve replicated measurements on an automatic Vickers Microhardness tester (Model: MVH-I, Meta Tech Industries, Pune, India) at a load of 50 N and a loading time of 20 s. The average value of the ﬁve replicated measurements of hardness is adopted as the microhardness value of the specimens. Unlubricated pin-on-disc sliding wear tests were carried out in order to determine the tribological properties of the nanocomposites. The disc material is made up of En-32 steel (diameter 160 mm and 8 mm thickness) having hardness value of HRc 65. The surface roughness of the disc varies from 0.02 to 0.06 lm. A constant 80 mm track diameter was used throughout the experimental work. The counterface slid against the BMI composite sample. Sliding was performed in air with the ambient temperature of around 25 °C over a period of 1 h at a sliding velocity of 0.84 m/s and a normal load of 40 N. Prior to wear testing, all specimens were cleaned, that is, the sample was abraded with water–abrasive paper (600 grit), a super-ﬁne water–abrasive paper, and liquid diamond polishing agent, successively. Then both the steel ring and the specimen were cleaned with acetone and distilled water. After that the steel ring and the specimen were dried at 70 °C. The friction force was measured using a torque shaft equipped with strain gauges, and the friction coefﬁcient was calculated automatically by taking into account the normal load and the friction force. The wear process takes some material away from the sample. This mass loss can accurately be measured by determining the weight of the specimen before and after the experiment. A characteristic value, which describes the wear performance under the chosen conditions for a tribo-system is the speciﬁc wear rate (Ks):
Ks ¼ Fig. 3b. Post curing cycle (oven temperature).
The zirconia represents the ceramic nanocrystalline phase and consists of primary particles in the size range of 60–100 nm (Fig. 2). Along with a spherical shape, their large number is characterized by a very high speciﬁc surface area of 100 m2/g. The nanoparticles are provided as a dry powder. This powder contains particle agglomerates with sizes in the micrometer range (Fig. 2), which consist of ZrO2 primary nanoparticles sticking strongly together. Primary nanoparticles attract each other due to adhesive inter-particle ‘van der Waals’ forces, which originate from the materials’ surface energy.
Dm mm3 q F N L Nm
where Dm is the mass loss, q is the measured density of the composite, FN is the normal load applied, and L is the sliding distance. In order to take repeatability into account, results from the friction and wear tests were obtained from three readings and the average value was adapted in our results. Scanning electron microscopy examinations on a Jeol-5400 was used to study the morphology of worn surfaces. Before observation, the surface of the sample was sprayed with an even thin ﬁlm of gold powder to improve the conductivity of the surface. The aim was to get information about the inﬂuence of ﬁllers on the corresponding wear mechanisms. 3. Results and discussion
2.2. Preparation of ZrO2 ﬁlled BMI nanocomposites 3.1. Effects of concentrations of ZrO2 on the microhardness Appropriate content of zirconia nanoparticles were added into BA at room temperature (25 °C) with vigorous mechanical agitating. The mixture was agitated for 2 h followed by ultrasonic
Generally, the microhardness of a material has close relationship with the tribological behaviour of the material. So it is necessary to
R.V. Kurahatti et al. / Materials and Design 32 (2011) 2644–2649
Fig. 4. Microhardness of neat BMI and nano-zirconia ﬁlled BMI composites.
study the effects of content of ZrO2 nanoparticles on the microhardness of the nanocomposites. As shown in Fig. 4, the Hv microhardness readings increased all the way from 57 of the neat BMI polymer to 68 in the 10 wt.% of nano-ZrO2 ﬁlled BMI composites, implying a maximum increment of 19%. It has been shown that a composite with a higher hardness value will be accompanied with lower wear rate and friction coefﬁcient . Note that the hardness increment is more signiﬁcant up to 5 wt.% of ﬁller loading. The higher Hv for 5 wt.% ﬁlled BMI composite is thought to result partly from the intrinsic hardness of ZrO2 and these nano particles might impose better resistance against BMI segment motion under indentation. However, further loading of ﬁller from 5 to 10 wt.%, the increase in hardness is very marginal suggesting that higher ﬁller loading gives rise to poor dispersion and agglomeration in the BMI matrix. Further, it might not be able to elaborate their full strengthening capability in hardness improvement. It seems that the 5 wt.% nano-ZrO2 particles could be more uniformly distributed and contributed the continuous hardness improvement. 3.2. Effects of concentration of ZrO2 on the speciﬁc wear rate and friction coefﬁcient In general, the friction and wear properties do always describe the whole tribological system rather than a material property alone. Fig. 5 shows the speciﬁc wear rate (Ks) of the nanocomposites as a function of nano-ZrO2 particle content. It was found that the nano-ZrO2 ﬁlled BMI composite exhibited a decreased Ks in comparison to the neat BMI. However, the Ks of the composites were not linearly related to the content of nano-ZrO2 content. The Ks sharply decreased when nano-ZrO2 content was below 1 wt.%. With the nano-ZrO2 content between 1 and 5 wt.%, the Ks decreased slightly with the increasing nano-ZrO2 content. The lowest speciﬁc wear rate was obtained with the nano-ZrO2-BMI composite containing 5 wt.%. Although, the Ks increased with increasing nano-ZrO2 above 5 wt.%, it was still lower in comparison
Fig. 5. Speciﬁc wear rate of neat BMI and nano-zirconia ﬁlled BMI nanocomposites.
to neat BMI. Among the ﬁlled nanocomposites, 5 wt.% nano-ZrO2 ﬁlled BMI showed the lowest speciﬁc wear rate. Rong et al.  examined the inﬂuence of microstructure on the tribological performance of nanocomposites by different compounding methods. They conformed that the dispersion state of the nanoparticles and micro-structural homogeneity of the ﬁllers improve the wear resistance signiﬁcantly. When the micro-structural homogeneity of the nanocomposites was improved, their wear resistance could be increased signiﬁcantly. The phenomenon reported in the present work is similar to what is reported in Ref. . However, a further increase in ﬁller loading leads obviously to a deterioration of the speciﬁc wear rate. A change in wear mechanism could be involved which may be ascribed to the large amount of hard ceramic nano-ZrO2 particles causing a higher abrasive wear. Some aspects of the reinforcing role that ceramic microparticles can play in the tribological behaviour were studied by Durand , who found that large particles protect the matrix better than smaller ones because they can shield the polymer if they are not pulled out. Small particles, on the other hand, were removed and then involved in an abrading wear process. Some important characteristics of nanocomposites have to be considered in order to explain this phenomenon. The quality of the interface in nanocomposites, usually play a very vital role in the materials capability to transfer stresses and elastic deformation from the matrix to the ﬁllers . If the ﬁller matrix interaction is poor, the nanoparticles are unable to carry any part of the applied load. In that case, the wear resistance cannot be greater than that of neat polymer matrix. If the bonding between the polymer matrix and ﬁllers is instead strong enough, the yield strength of the ﬁlled composite can be higher than that of the neat matrix . In the same way, the difference in reducing the friction coefﬁcient and improving the wear resistance ability of neat BMI and nanoZrO2 ﬁlled BMI composites should result mainly from the adhesion strength of the ﬁller-matrix. Based on the experience from various studies, Friedrich et al.  concluded that ﬁne particles contribute better to the property improvement under sliding wear conditions than larger particles. A similar trend was conﬁrmed by Xing and Li  recently on the spherical silica particles ﬁlled epoxy when particle size varied from 120 to 510 nm. In the present work, the results are showing the similar trend. Besides improving the wear resistance, the nanoparticles also reduce the coefﬁcient of friction as shown in Fig. 6. Evidently, the nanocomposites with 5 wt.% nano-ZrO2 ﬁlled BMI has the lowest friction coefﬁcient. The coefﬁcient of friction of 5 wt.% nano-ZrO2 ﬁlled BMI nanocomposite is 0.62 that amounts to 82% of the neat BMI matrix. Detachment of the nanoparticles and small amount of the surrounding matrix plays the main role in the material removal due to wear. The detached nanoparticles might also act as solid lubricants. These account for the lower speciﬁc wear rates and friction coefﬁcients of the nanocomposites.
Fig. 6. Coefﬁcient of friction of neat BMI and nano-zirconia ﬁlled BMI nanocomposites.
R.V. Kurahatti et al. / Materials and Design 32 (2011) 2644–2649
Fig. 7. Worn surface features of (a) neat BMI, (b) 5 wt.% nano-zirconia ﬁlled BMI, and (c) 10 wt.% nano-zirconia ﬁlled BMI nanocomposites.
3.3. Worn surface morphology Observations of the worn surfaces by scanning electron microscope (SEM) provide knowledge about both, the role that nanoparticles play in the reduction of wear rate, and the wear mechanisms. Some wear pattern representatives for each sample are displayed in Fig. 7a–c. Main features on the worn surface of the neat BMI resin are severe damage characterized by the disintegration of the top surface, wear debris and deep grooves in the sliding direction (Fig. 7a). Polymer fragments of the size of micrometers detach and leave small craters behind. These polymer fragments, which might be captured between the counterface and the pin sample, abrade the sample surface leading to even more substantial loss of material. In the case of ﬁlled nanocomposites, the appearances are completely different and become rather smooth. Although the ploughing grooves are still visible on the nanocomposite sample surface, the groove depths are shallow on 5 wt.% ﬁlled BMI (Fig. 6) and at some region, the grooves are simply invisible (Fig. 7b). It seems the low ﬁller loading is insufﬁcient and cannot bring about significant improvements in wear resistance (Fig. 5). The wear performance of a composite material is indeed known to be volumetric dependent. It is noted that some cracks across the wear tracks are visible on the composites’ worn surface (Fig. 7b). Very ﬁne scratches are visible resulting from the nano-ﬁllers pulled out of the matrix, and then further moved across the surface by scratching and rolling. Thus, it can be concluded that the abrasive wear of neat BMI is replaced by fatigue wear when the nanoparticles are
introduced. Due to their size, the particles should be able to move into gaps in the counterface and may then be exposed to rolling rather than sliding/scratching movement. Large matrix fragments are not found. During sliding, a rolling effect of nanoparticles could reduce the shear stress, the friction coefﬁcient, and the contact temperature. The matrix damages in the interfacial region were reduced by this rolling effect. This process probably plays a key role to the reduced friction coefﬁcient. Further, the ability of nano-ZrO2 to improve the tribological behaviour is increased with decreasing the particle size of nanometer ZrO2. The wear rate of larger particle size ZrO2-ﬁlled PEEK was high because the composite transfer ﬁlm had poor adhesion to the counterface . On the other hand, in the present work, the wear–resistant BMI composite which was ﬁlled with small size ZrO2 particles (<70 nm) transferred well to the counterface and its transfer ﬁlm was thin, uniform and adhered strongly to the counterface. Thus the improvement in the tribological behaviour of nanometer ZrO2ﬁlled BMI composite is related to the improved characteristics of the transfer ﬁlm. However, the wear resistance suffers if the ﬁller loading exceeds 5 wt.% and the large amount of nanoparticles cannot provide any wear reducing effect. Abrasive wear is accompanied by delamination and fatigue cracking of the matrix (Fig. 7c).
4. Conclusions This study focused on the development of nanocomposites with properties superior to the neat matrix. The following conclusions can be drawn:
R.V. Kurahatti et al. / Materials and Design 32 (2011) 2644–2649
The addition of nano-ZrO2 particles increases the hardness of BMI nanocomposites. The tribological performance of the composites showed a good correlation with the hardness up to 5 wt.% of ﬁller loading. Based on microscopic observations of the worn surfaces, a positive rolling effect of the debris (matrix and nanoparticles) between the sample and the counterface, which led to remarkable reduction of friction coefﬁcient. This effect becomes more remarkable when the nano-ZrO2 content is 5 wt.%. The wear resistance of BMI nanocomposites considerably increases with increasing content of ZrO2. The wear-resistant BMI composite which was ﬁlled with small size ZrO2 particles (<70 nm) transferred well to the counterface and its transfer ﬁlm was thin, uniform and adhered strongly to the counterface. Thus the improvement in the tribological behaviour of nanometer ZrO2-ﬁlled BMI composite is related to the improved characteristics of the transfer ﬁlm. An optimum wear resistant composition was found to be BMI with 5 wt.% nano-ZrO2 particles. Nano-ZrO2 ﬁlled BMI nanocomposites show signs of mild abrasive wear due to the hard ceramic particles. The main wear mechanism of composite changed from the severe abrasive wear (for neat BMI matrix) to mild abrasive wear.
Acknowledgments Mr. R.V. Kurahatti is thankful to Dr. K.U. Bhasker Rao, Director DMSRDE for permitting to conduct part of Ph.D. Research work in DMSRDE. Dr. Nirbhay Singh, Dr. A V Ramesh Kumar and Saurabh Srivastava are thankful to Dr. K U Bhasker Rao, Director, DMSRDE for his help and encouragement. References  Zhang Z, Breidt C, Chang L, Haupert F, Friedrich K. Enhancement of wear resistance of epoxy: short carbon ﬁber, graphite, PTFE and nano-TiO2. Compos Part A 2004;35:1385–92.  Chang L, Zhang Z. Tribological properties of epoxy nanocomposites. Part II, a combinative effect of short carbon ﬁbers with nano-TiO2. Wear 2006;260:869–78.  Ng CB, Schadler LS, Siegel RW. Synthesis and mechanical properties of TiO2epoxy nanocomposites. Nanostruct Mater 1999;12:507–10.  Rong MZ, Zhang MQ, Liu H, Zeng HM, Wetzel B, Friedrich K. Microstructure and tribological behavior of polymeric nanocomposites. Ind Lubr Tribol 2001;53(2):72–7.
 Zhang MQ, Rong MZ, Yu SL, Wetzel B, Friedrich K. Improvement of tribological performance of epoxy by the addition of irradiation grafted nano-inorganic particles. Macromol Mater Eng 2002;287:111–5.  Zhang MQ, Rong MZ, Yu SL, Wetzel B, Friedrich K. Effect of particle surface treatment on the tribological performance of epoxy based nanocomposites. Wear 2002;253:1088–95.  Wang Q, Xue Q, Liu W, Shen W, Xu J. The effect of particle size of nanometer ZrO2 on the tribological behaviour of PEEK. Wear 1996;198:216–9.  Yan H-X, Ning R-C, Ma X-Y, Zhang Q-Y. Friction and wear behavior of nanometer Si3N4-ﬁlled bismaleimide composites. Tribology 2001;21(6):452–5 [in Chinese].  Bauer F, Sauerland V, Gläsel H, Ernst H, Findeisen M, Hartmann E, et al. Preparation of scratch and abrasion resistant polymeric nanocomposites by monomer grafting onto nanoparticles: effect of ﬁller particles and grafting agents. Macromol Mater Eng 2002;287:546–52.  Wetzel B, Haupert F, Friedrich K, Zhang MQ, Rong MZ. Impact and wear resistance of polymer nanocomposites at low ﬁller content. Polym Eng Sci 2002;42:1919–27.  Harsha AP, Tewari US, Venkataraman B. Three-body abrasives wear behaviour of polyaryletherketone composites. Wear 2003;254:680–92.  Suresha B, Chandramohan G, Siddaramaih, Jayaraju T. Three body abrasive wear behavior of E-glass ﬁber reinforced/graphite-ﬁlled epoxy composites. Polym Compos 2008;29:631–7.  Singh RP, Zhang M, Chan D. Toughening of a brittle thermosetting polymer: effects of reinforcement particle size and volume fraction. J Mater Sci 2002;37:781–8.  Wetzel B, Haupert F, Friedrich K, Zhang MQ, Rong MZ. Mechanical and tribological properties of microparticulate and nanoparticulate reinforced polymer composites. In: Proceedings of the 13th ECCM, 2001, Brugge, Belgium.  Hussain M, Nakahira A, Niihara K. Fracture behavior and fracture toughness of particulate ﬁlled epoxy composites. Mater Lett 1996;26:185–91.  Yan YH, Shi XM, Liu JG, Zhao T, Yu YZ. Thermosetting resin system based on novolac and bismaleimide for resin transfer molding. J Appl Polym Sci 2002;83:1651–7.  Choudhari M, Galvin T, King J. Characterization of bismaleimide system. XU 292. SAMPE J 1985;21:27.  Lin TK, Wu SJ, Lai JG, Shyu SS. The effect of chemical treatment on reinforcement/matrix interaction in Kevlar-ﬁber bismaleimide composites. Comp Sci Techn 2000;60:1873–6.  Liu L, Gu A, Fang Z, Tong L, Xu Z. The effects of the variations of carbon nanotubes on the micro-tribological behavior of carbon nanotubes/ bismaleimide nanocomposites. Compos Part A 2007;38:1957–8.  Wang QH, Xu J, Shen W, Liu W. An investigation of the friction and wear of nanometer Si3N4 ﬁlled PEEK. Wear, 1996;196:82–6.  Durand JM, Vardavoulias M, Jeandin M. Role of reinforcing ceramic particles in the wear behaviour of polymer-based model composites. Wear 1995;181– 183:833–9.  Zhang M, Zeng H, Zhang L, Lin L, Lin G, Li RKY. Fracture characteristics of discontinuous carbon ﬁber-reinforced PPS and PESC composites. Polym Compos 1993;1:357–65.  Wu CL, Zhang MQ, Rong MZ, Friedrich K. Tensile performance improvement of low nanoparticles ﬁlled-polypropylene composites. Compos Sci Technol 2002;62:1327–40.  Friedrich K, Zhang Z, Schlarb AK. Effect of various ﬁllers on the sliding wear of polymer composites. Compos Sci Technol 2005;65:2329–43.  Xing XS, Li RKY. Wear behaviour of epoxy matrix composites ﬁlled with uniform sized sub-micron spherical particles. Wear 2004;256:21–6.